Structure and physical properties of single crystal PrCr2Al20 and CeM2Al20 (M=V, Cr): A comparison of compounds adopting the CeCr2Al20 structure type
Kangas, Michael J.; Schmitt, Devin C.; Sakai, Akito; Nakatsuji, Satoru; Chan, Julia Y.; Journal of Solid State Chemistry 196 (2012) 274–281; doi:10.1016/j.jssc.2012.06.035

data_1562866
_publ_section_title
;
 Structure and physical properties of single crystal PrCr2Al20 and
 CeM2Al20 (M=V, Cr): A comparison of compounds adopting the CeCr2Al20
 structure type
;
_journal_name_full               'Journal of Solid State Chemistry'
_journal_page_first              274
_journal_page_last               281
_journal_paper_doi               10.1016/j.jssc.2012.06.035
_journal_volume                  196
_journal_year                    2012
_chemical_formula_moiety         'Al20 Ti2 Yb'
_chemical_formula_sum            'Al20 Ti2 Yb'
_chemical_formula_weight         808.44
_space_group_IT_number           227
_space_group_name_Hall           '-F 4vw 2vw 3'
_space_group_name_H-M_alt        'F d -3 m :2'
_symmetry_cell_setting           cubic
_symmetry_space_group_name_H-M   'F d -3 m :2'
_atom_sites_solution_primary     direct
_atom_sites_solution_secondary   difmap
_audit_creation_method           SHELXL-97
_cell_angle_alpha                90.00
_cell_angle_beta                 90.00
_cell_angle_gamma                90.00
_cell_formula_units_Z            8
_cell_length_a                   14.6890(18)
_cell_length_b                   14.6890(18)
_cell_length_c                   14.6890(18)
_cell_measurement_reflns_used    381
_cell_measurement_temperature    298.0(5)
_cell_measurement_theta_max      29.131
_cell_measurement_theta_min      2.546
_cell_volume                     3169.4(7)
_computing_structure_refinement  'SHELXL-97 (Sheldrick, 2008)'
_diffrn_ambient_temperature      298.0(5)
_diffrn_measured_fraction_theta_full 0.996
_diffrn_measured_fraction_theta_max 0.996
_diffrn_measurement_device_type  'Nonius KappaCCD'
_diffrn_measurement_method       '\w and \f scans'
_diffrn_radiation_monochromator  graphite
_diffrn_radiation_source         'fine-focus sealed tube'
_diffrn_radiation_type           MoK\a
_diffrn_radiation_wavelength     0.71073
_diffrn_reflns_av_R_equivalents  0.0477
_diffrn_reflns_av_sigmaI/netI    0.0412
_diffrn_reflns_limit_h_max       20
_diffrn_reflns_limit_h_min       -19
_diffrn_reflns_limit_k_max       14
_diffrn_reflns_limit_k_min       -14
_diffrn_reflns_limit_l_max       13
_diffrn_reflns_limit_l_min       -13
_diffrn_reflns_number            688
_diffrn_reflns_theta_full        29.10
_diffrn_reflns_theta_max         29.10
_diffrn_reflns_theta_min         3.92
_exptl_absorpt_coefficient_mu    7.926
_exptl_absorpt_correction_T_max  0.5697
_exptl_absorpt_correction_T_min  0.5697
_exptl_absorpt_correction_type   multi-scan
_exptl_absorpt_process_details   'HKL Scalepack (Otwinowski & Minor 1997)'
_exptl_crystal_colour            grey
_exptl_crystal_density_diffrn    3.389
_exptl_crystal_density_method    'not measured'
_exptl_crystal_description       cubic
_exptl_crystal_F_000             2992
_exptl_crystal_size_max          0.08
_exptl_crystal_size_mid          0.08
_exptl_crystal_size_min          0.08
_refine_diff_density_max         1.032
_refine_diff_density_min         -1.662
_refine_diff_density_rms         0.175
_refine_ls_extinction_coef       0.0041(3)
_refine_ls_extinction_expression Fc^*^=kFc[1+0.001xFc^2^\l^3^/sin(2\q)]^-1/4^
_refine_ls_extinction_method     SHELXL
_refine_ls_goodness_of_fit_ref   1.190
_refine_ls_matrix_type           full
_refine_ls_number_parameters     17
_refine_ls_number_reflns         241
_refine_ls_number_restraints     0
_refine_ls_restrained_S_all      1.190
_refine_ls_R_factor_all          0.0350
_refine_ls_R_factor_gt           0.0280
_refine_ls_shift/su_max          0.000
_refine_ls_shift/su_mean         0.000
_refine_ls_structure_factor_coef Fsqd
_refine_ls_weighting_details
'calc w=1/[\s^2^(Fo^2^)+(0.0346P)^2^+0.0000P] where P=(Fo^2^+2Fc^2^)/3'
_refine_ls_weighting_scheme      calc
_refine_ls_wR_factor_gt          0.0623
_refine_ls_wR_factor_ref         0.0670
_reflns_number_gt                222
_reflns_number_total             241
_reflns_threshold_expression     I>2\s(I)
_cod_data_source_file            JSSC-2012-196-274.cif
_cod_data_source_block           YbTi2Al20
_cod_depositor_comments
;
The following automatic conversions were performed:

data item '_symmetry_cell_setting' value 'Cubic' was changed to
'cubic' in accordance with the built-in table derived from the CIF
Core dictionary named 'cif_core.dic' version 2.4.5 last updated on
2014-11-21.

Automatic conversion script
Id: cif_fix_values 8369 2020-08-20 11:38:08Z andrius 
;
_cod_original_sg_symbol_H-M      'F d -3 m      '
_cod_database_code               1562866